Aqueous polymerization of vinyl monomers
in the presence of surfactants
IV. Effect of the chain length of the surfactant on the acrylamide
V. VAŠKOVÁ, V. JURANIČOVÁ, and J. BARTOŇ
Polymer Institute, Centre for Chemical Research,
Slovak Academy of Sciences, CS-842 36 Bratislava
Received 2 October 1985
Dedicated to Professor Ing. A. Hrivík, CSc., in honour of his 60th birthday
The kinetics of acrylamide polymerization in water initiated by (NH^ÄOg
was studied in presence of the surfactants C8H17S03Na, C12H25S04Na, and
Ci6H33S04Na. In the presence of the surfactants an increase in the acrylamide
polymerization rate and decrease in the degree of polymerization was obser
ved. At concentrations above critical micellar concentration the surfactant
C12H25S04Na causes a gentle decrease of the overall activation energy of
acrylamide polymerization. The length of the n-alkyl chain in the surfactant
molecule does not influence the acrylamide polymerization rate.
Изучена кинетика полимеризации акриламида в воде, инициируемая
(NH4)2S208, в присутствии поверхностно-активных веществ C8H17S03Na,
Ci2H25S04Na и C16H33S04Na. В присутствии поверхностно-активных ве
ществ наблюдалось увеличение скорости полимеризации акриламида при
одновременном понижении степени полимеризации. При концентрациях
высших, чем критическая мицеллярная концентрация, ПАВ C12H25S04Na
вызывает некоторое снижение полной энергии активации полимеризации
акриламида. Длина н-алкильной цепи в молекуле ПАВ не влияет на
скорость полимеризации акриламида.
In the studies on the kinetics and mechanism of acrylamide polymerization the
authors  reported that in the presence of an anionic emulsifier in the concentra
tion range above its critical micellar concentration (c.m.c.) an increase in the
acrylamide polymerization rate was observed. At the same time, the nonionic
emulsifier isooctylphenoxy polyethoxy ethanol did not affect the acrylamide
polymerization rate at all. A cationic emulsifier cetyltrimethylammonium bromide
caused even a decrease in the acrylamide polymerization rate. Similar results were
mentioned by Kim et al.  in the kinetics study of the acrylamide polymerization.
In our earlier papers [3, 4] we reported on the effect of the emulsifier and/or
poly(butyl acrylate) latex on the homogeneous acrylamide polymerization initiated
Chem. Papers 40 (4) 435-^41 (1986) 435
V. VAŠKOVÁ, V. JURANIČOVÁ, J. BARTOŇ
by water-soluble initiators. It was found that the commercial emulsifier Dow-
fax 2A1 (sodium dodecylphenoxybenzenedisulfonate) did not affect the ac-
rylamide polymerization rate. It worked only as an effective chain transfer agent
. In the presence of poly(butyl acrylate) latex, however, an increase of the
acrylamide polymerization rate was observed. That was believed to be a consequ
ence of the simultaneous grafting to the poly(butyl acrylate) latex with acrylamide
The aim of the present study is to find out the influence of the chain length of the
alkyl substituent of the anionic surfactants on the aqueous acrylamide polymeriza
tion initiated by water-soluble initiator ammonium peroxodisulfate.
Anal, grade ammonium peroxodisulfate (Merck—Schuchard), acrylamide (Merck—
—Schuchard), and the surfactants (Merck—Schuchard) were used as supplied. The surfac
tants used were: sodium octanesulfonate, sodium dodecyl sulfate, and sodium hexadecyl
sulfate, all chemicals for tenside research. Sodium hydrogen sulfate monohydrate was an
anal, grade chemical. The polymerization medium water was distilled and then deaerated by
boiling and bubbling with argon before use.
Polymerization was carried out under a stream of argon at given polymerization
temperature. Monomer acrylamide, surfactant, and water were charged into the reaction
vessel. The reaction mixture was then thermostated under an argon stream to the
temperature of polymerization. The aqueous solution of initiator was then injected into the
polymerization system. Gravimetric determination of conversion and the isolation of
polymer from the reaction product have already been described in detail elsewhere [3, 4].
The limiting viscosity numbers of the polymer [rj] were established in water at 30 °C.
According to the procedure , the viscosity average relative molecular mass, (M,),,, of
Polyacrylamide was calculated according to the relation
3kg-1) = 6.31xlO- 4(M r)r (1)
(Мг)„ was converted to number average relative molecular mass (Mr)N according to the
relation (2) valid when termination occurs via disproportionation
Ä = r ( a + 2 ) (2)
where Г is the gamma function and a is the exponent in relation (1) equal to 0.8.
Absorption spectra of the initiator and surfactant solutions were measured on the
Beckmann UV spectrophotometer at 25 °C.
436 Chem. Papers 40 (4) 435—441 (1986)
POLYMERIZATION OF VINYL MONOMERS. IV
Results and discussion
The effect of the type and of the concentration of the emulsifier on the
acrylamide polymerization rate is summarized in Table 1. As shown the surfactants
C8Hi7S03Na, C12H25S04Na, and C^H^SC^Na increase the rate of acrylamide
polymerization. It is reasonable to assume that the SO!" as well as SO?" groups are
not responsible for the increase of the polymerization rate, Which follows from the
results obtained for the acrylamide polymerization rate in the presence of NaHS03
and NaHS04 in a concentration range from 10~
3 to 10"1 mol dm"3. Under these
conditions the acrylamide polymerization rate remains practically unaffected. For
the surfactant C^ftsSC^Na a c.m.c. value of 9 x 10"3 mol dm"3 was established at
20 °C. As seen from Fig. 1 the increase of the acrylamide polymerization rate is
evident at surfactant concentrations under as well as above c.m.c. In Fig. 2 is
illustrated the dependence of the logarithms of the acrylamide polymerization rate
on the logarithms of the surfactant concentrations for all three surfactants studied.
Initial acrylamide polymerization rates jRpo and degrees of polymerization PN in argon atmosphere at
the temperature of 50 °C in the presence of the surfactants E, initiated by ammonium peroxodisulfate
(c = 5xl0- 4 moldm- 3 )
[AAM]o = 0.5moIdm-3
p N -io-
* Estimated for samples with the mass conversion under 20 %.
Chem. Papers 40 (4) 435—441 (1986) 4 3 7
mol dm - 3
mol dm - 3 s - 1
V. VAŠKOVÁ, V. JURANIČOVÁ, J. BARTOŇ
From the results obtained it can be deduced that the increase in the acrylamide
polymerization rate is influenced only by the surfactant concentration but not by
the length of the surfactant n-alkyl substituent chain. From the plot in Fig. 2
obtained formal reaction order to the surfactant for all three surfactants studied is
10 20 30 40 ť/min
Fig. 1. Dependence of the acrylamide conversion on the surfactant Ci2H25S04Na ([E]0) concentration.
Reaction temperature 50 °C, [AAM]0 = 0.5 mol dm
-3, [(NH4)2S208]o = 5 x 10"
4 mol dm- 3.
a) Without surfactant; b) [E]0 = 5 x 10
-4 mol dm - 3; c) [E]0 = 5 x 10
-2 mol dm- 3.
- ^ ̂ " #
log ([£"]/(mol dm"3)) • 4
Fig. 2. Dependence of the logarithms of the initial acrylamide polymerization rate R^ on the logarithms
of the initial surfactants concentration. Reaction temperature 50 °C, [(NKibSzOeb =
= 5 X lO"4 mol dm"3, [AAM]0 = 0.5 mol dm"
О CsHnSOaNa; • C12H25S04Na; Э C16H33S04Na.
438 Chtth. Papers 40 (4) 435—441 (1986)
POLYMERIZATION OF VINYL MONOMERS. IV
For explanation of the influence of the surfactants on the course of the
acrylamide polymerization in water the interaction in the system initiator—
—surfactant was studied. For this purpose the absorption spectra of the initiator
and surfactant C12H25S04Na solution in UV region were analyzed (Fig. 3). After
mixing both components together no new absorption band is formed, but the
intensity of the surfactant absorption band with a maximum at 200 nm decreases
proportionally to the concentration of the initiator added. The maxima of the
absorption band are simultaneously shifted towar